Study of interfacial adhesion energy of multilayered ULSI thin film
structures using four-point bending test
Zhenghao Gan a, *, S.G. Mhaisalkar a , Zhong Chen a , Sam Zhang b , Zhe Chen c , K. Prasad c
a School of Materials Engineering, Nanyang Technological University, Singapore 639798, Singapore
b School of Mechanical and Production Engineering, Nanyang Technological University, Singapore 639798, Singapore
c School of Electrical and Electronic Engineering, Nanyang Technological University, Singapore 639798, Singapore
Available online 19 November 2004
Adhesion between barrier layers and interconnect metals or dielectrics continues to be a significant concern in the microelectronic
industry, with delamination occurring in between the layers leading to device failure. As the sizes of transistors are scaled down to submicron
regime, new materials and multilayered thin film structures are applied, which pose a great challenge to quantify the adhesion energy of the
interfaces in order to optimize the structures of the multilayered thin films. In this paper, the four-point bending technique is used to quantify
the adhesion energy ( G c) between interfaces in multilayered thin film structures for ULSI. An example is presented to demonstrate the
applicability of the four-point bending technique for determining the adhesion strength of the SiC/porous polyarylene ether (PAE)/SiC
interface. The Gc value obtained is 26.2 J/m 2 , higher than that of the SiN/PAE interface reported by others, indicating a good adhesion. The
resulting fracture surfaces were then characterized by field emission scanning electron microscopy (FESEM) and X-ray photoelectron
spectroscopy (XPS) to identify the location of the debonded path. It is found that the crack propagates alternatively between the two PAE/SiC
D 2004 Elsevier B.V. All rights reserved.
PACS: 68.35.Np; 68.37.Hk; 68.49.Uv; 81.05.-t
Keywords: Four-point bending; Photoelectron microscopy; Silicon carbide; Polyarylene ether (PAE)
With the continuous reduction of circuit sizes, reliability
continues to pose serious challenges in advanced microelectronic
applications. The challenges mainly arise from
the application of new materials such as copper and porous
low-k and multilayered thin film structures.
It is believed that the reliability of Cu metallization is
correlated to the interfacial adhesion strength of the multilayer
thin film structures. Lane et al.  presented a linear
relationship between the electromigration (EM) activation
energy and the intrinsic work of adhesion. Debonding most
likely occurs at the weak interfaces during processing and
device operation. The debonding driving force may include
* Corresponding author. Tel.: +65 67906343; fax: +65 67909081.
E-mail address: firstname.lastname@example.org (Z. Gan).
Surface & Coatings Technology 198 (2005) 85–89
0257-8972/$ - see front matter D 2004 Elsevier B.V. All rights reserved.
the residual stress generated during deposition and thermal
stress arisen from the mismatch of thermal expansion
coefficients among different layers. The occurrence of
decohesion basically depends on the competition between
the debonding driving force and the interfacial adhesion
strength. Therefore, there is a strong need to characterize
and quantify the interfacial adhesion strength.
Research on low-k dielectrics has been actively conducted
to look into different materials that are able to meet
the requirements for Cu-damascene processing. Basically,
low-k films could be categorized into two groups based on
film composition and deposition method. One is low-k with
Si–O structures deposited by CVD method. The other group
has C–C chemical structure and deposited by spin-on
method such as polyarylene ether (PAE).
For the first group, the adhesion strength measurement for
carbon-doped oxides (SiOC)/Si interface was given elsewhere
. For the second group, a preliminary study on SiC/
Fig. 1. Multi-stack of the SiC/PAE/SiC/USG thin films under study.
PAE interfacial adhesion strength is presented here. It was
recently reported  that an amorphous hydrogenated SiC (a-
SiC:H)/Ta dielectric/metal bilayer sidewall diffusion barrier
could be applied to improve the electrical performance of Cu/
porous ultralow-k (porous-PAE) interconnects by increasing
the electrical breakdown field (EBD). This improvement was
initially attributed to the sealing effect of a-SiC:H on the
porous low-k material.
The interfacial adhesion strength is commonly characterized
by the critical energy release rate ( G c). Four-point
bending test can give quantitative Gc, whereby the results
obtained are reproducible. It is well established  that Gc is a
function of phase angle of mixed-mode stress intensity (W),
W ¼ arctgðKII=KIÞ ð1Þ
where KI and KII denote the Mode I and Mode II stress
intensity factors. W varies from 08 to 908, corresponding to
pure Mode I and pure Mode II, respectively.
The fracture mode at an interface of dissimilar materials
is often mixed (i.e., 08bWb908), mainly caused by the
mismatch of material properties such as elastic properties
and thermal expansion coefficients. In practice, the typical
phase angle involved in many delamination phenomena
ranges between 08 and 508 . The phase angle of the
mixed-mode stress intensity for four-point bending is
around 458 . In other words, Gc given by the fourpoint
bending is an upper bound of the practical interfacial
Another unique characteristic of four-point bending is
that the thin films are sandwiched between two
elastically massive substrates (such as Si wafer) during
test, and the relaxation of residual stress is confined,
compared to other commonly employed techniques such
as scotch tape test , scratch test, indentation test and
peel test .
In this paper, four-point bending technique will be
applied to quantify the interfacial adhesion energy of the
Z. Gan et al. / Surface & Coatings Technology 198 (2005) 85–89
SiC/PAE interface in a multilayered thin film structure (SiC/
A multi-stack of thin films shown in Fig. 1 was
produced to study the SiC/PAE interfacial adhesion
strength. The thin film stack was prepared on 8-in.diameter
p-type Si(100) wafers. A 800-nm-thick blanket
film of undoped silicate glass (USG) was first deposited
on the clean Si wafer by PECVD technique in an Applied
Material Centurak 5200 PECVD system. The precursors
used for USG deposition are silane (SiH4) and nitrous
oxide (N2O). The 50-nm-thick a-SiC:H film (named here
as: SiC1) was then deposited in the same PECVD system
using trimethylsiane. PAE layer with a thickness of 300
nm was then spun onto the wafer. Another a-SiC:H
surface layer (named here as: SiC2) was deposited to
protect the PAE.
To produce specimens for four-point bending test (Fig.
1), the silicon wafer coated with the above-mentioned
film stacks (SiC1/PAE/SiC2/USG) were diced into rectangular
pieces of sizes of 46 7 mm and were then
glued to bare silicon with an epoxy. The individual fourpoint
bend specimens were centrally notched with a
precision cutter to within ~100 Am to the thin film
interface. This is to ensure that the crack can propagate
into the interfaces, rather than penetrate into the massive
Fig. 2 gives a schematic setup for four-point bending
test. The specimen is tested using four-point bending with
loading rate around 0.05 Am/s. The loads are measured to
0.01 N resolution and digitally recorded to generate the
load–displacement curve. When the load is high enough,
a pre-crack will initiate from the pre-notch and propagate
perpendicularly toward the interface in the thin film
stack, and can grow longitudinally along the weakest
interface. Mechanics of interface cracks  indicate that,
sufficiently far away from the pre-notch, the crack
propagates along the weakest interface at a constant
load, corresponding to steady propagation. The constant
Fig. 2. Schematic setup for four-point bending test.
Fig. 3. Load–displacement curves for three independent specimens.
load ( Pc) is independent of the crack length, and is related to
Gc as follows :
Gc ¼ 31 m22 P2 cL2 2E2b2h3 1
2 g3 1 þ kg3 2
2 þ 12k
1g2 g1 þ kg2 ð2Þ
where subscripts 1 and 2 denote substrates 1 and 2,
respectively; E and m are Young’s modulus and Poisson ratio
for the substrates; L is the distance between inner and outer
dowel pins; Pc is the load during steady propagation; b and h
are the width and half thickness of the sandwiched beam (i.e.,
h=(h1+h2)/2); and the nondimensional parameters are:
k ¼ E2= 1 m 2 2
E1= 1 m 2 1
gi ¼ hi
When the two substrates are of the same material and
with the same thickness (i.e., h1=h2=h), k=1, and g1=g2=1.
Eq. (2) is reduced to :
21ð1m2ÞP Gc ¼ 2 cL2 16Eb2h3 ð5Þ
To identify the location of the debonded path, the
morphology of the resulting fracture surfaces was observed
Z. Gan et al. / Surface & Coatings Technology 198 (2005) 85–89 87
by field emission scanning electron microscopy (FESEM)
(JEOL JSM-6340F, Japan). X-ray photoelectron spectroscopy
(XPS) measurements were carried out to investigate
interface chemistry on fracture surfaces in a Kratos AXIS
spectrometer (UK) with the monochromatic Al Ka X-ray
radiation at 1486.71 eV. The base vacuum in XPS analysis
chamber was about 10 9 Torr.
3. Results and discussion
Fig. 4. FESEM image of the bottom part fracture surface.
Fig. 3 gives the load–displacement curves for five
specimens. The initial slope of these curves represents the
stiffness of the specimen. Around 60 N loading force, crack
starts to grow into the weakest interface below the pre-notch
since there was a sudden drop of load, indicating a release of
stress or energy. The average interfacial fracture energy or
strain energy release rate G c for the five specimens using
Eq. (5) was calculated to be 26.2 J/m 2 . It is seen in Fig. 3
that the obtained Gc values are reproducible.
However, it is clear that the load–displacement curves
related to the longitudinal steady crack propagation are
uneven, showing a serrated shape. This is correlated to the
complicated crack propagation path, as evidenced by the
fractography of the fractured surfaces. Both PAE and SiC2
layers are observed in the SEM image of the bottom part of
the fractured surface (Fig. 4).
Fig. 5a shows the XPS survey spectrum of the bottom
part fractured surface. The peaks corresponding to Si 2p, Si
2s, C 1s and Auger, O 1s and Auger are obviously observed.
Fig. 5b gives the C 1s core-level spectrum of the bottom part
fractured surface, which can be curve-fitted with three peak
components with binding energies at 283.4, 285, and 286.3
eV, attributed to the C–Si bond , the C–C bond, and the
C–O bond , respectively. The latter two bonds are
commonly observed in the XPS spectrum of PAE . The
high resolution Si 2p spectrum of the same surface is plotted
in Fig. 5c, which is deconvoluted into three components
with binding energies centered at 100.5, 101.7, and 103.9
eV, contributed by the Si bonds in SiC, SiOC, and SiO2,
respectively . It is noted that the latter two species
(SiOC and SiO 2) appear due to the exposure of the
amorphous SiC in the delaminated interfaces to the air for
Fig. 5. (a) Survey, (b) C 1s and (c) Si 2p core-level spectrum of the bottom
part fracture surface.
some time . In other words, the XPS analysis supports
the SEM observation—part of PAE and part of SiC2 layers
are exposed after four-point bending test.
Based on the above XPS analysis and SEM examination, it
is thus concluded that the crack propagates alternatively
between the SiC1/PAE and PAE/SiC2 interfaces, as schematically
illustrated in Fig. 6. A detailed illustration is given
Z. Gan et al. / Surface & Coatings Technology 198 (2005) 85–89
as follows. The selected epoxy has a strong adhesion to the
top silicon wafer. The experimentally measured G c value for
epoxy/Si interface is 20 J/m 2 . When the crack advances to the
epoxy/SiC1 interface (point A), it will possibly propagate
into this interface if the SiC layer is strong enough.
Hutchinson  predicted that penetration is also likely if
the interface toughness exceeds about 1/4 of the toughness of
the material across the interface (i.e., SiC1 here). According
to the following equation (assuming plane stress):
Gc ¼ K2 c
the estimated Gc values for SiC and PAE layers are
approximately 40 and 160 J/m 2 , respectively, based on the
experimental E and Kc data reported by others [13,14]. As the
crack tip reaches the epoxy/SiC1 interface at point A, it will
penetrate into the SiC layer since the Gc of this interface is
higher than 1/4Gc of the SiC layer. Upon reaching the SiC1/
PAE interface at point B, the crack will grow along the
interface since the PAE layer is relatively tough. However,
with the further propagation of the crack along the SiC1/PAE
interface, the crack will likely penetrate into the PAE layer at
point C due to the presence of a high number of pores (or
defects) at the PAE/SiC interface. Following the crack
extension in PAE, it is deflected towards the PAE/SiC2
interface at point D. Thus, a new interfacial crack along the
PAE/SiC2 interface forms. The process is repeated, and
finally results in the alternating crack along the two
Since the crack propagates alternatively between the two
PAE/SiC interfaces, it is still a good approximation to use
the averaged serrated part of the load–displacement curves
to evaluate the critical energy release rate of the PAE/SiC
It is worth mentioning that the measured Gc value
obtained here for PAE/a-SiC:H interface is higher than that
of SiN/PAE interface reported by others . This
demonstrates that the a-SiC:H thin film could be a
promising layer to enhance the adhesion of PAE to other
materials, and thus enhance the reliability of future devices.
Fig. 6. Schematic crack propagation path (indicated by the arrows) during
four-point bending test of the specimen.
This paper has successfully demonstrated the capability
of the four-point bending technique in determining the
adhesion strength of an a-SiC:H/PAE interface in a
multilayered structure. FESEM observation and XPS
characterization have confirmed that during four-point
bending of such a structure, the crack propagates along a
unique path alternating in the two adjacent interfaces. The
critical energy release rate G c obtained for a-SiC:H/PAE
interface is 26.2 J/m 2 higher than that of SiN/PAE interface
reported by others. This demonstrates that the a-SiC:H thin
film could be a promising layer to enhance the adhesion of
PAE to other materials, and thus enhance the reliability of
The authors would like to thank the staffs in Department
of Silicon Process Technology, Institute of Microelectronics
(IME), for technical support and help in
Z. Gan et al. / Surface & Coatings Technology 198 (2005) 85–89 89
 M.W. Lane, E.G. Liniger, J.R. Lloyd, J. Appl. Phys. 93 (2003) 1417.
 J. Widodo, W. Lu, S.G. Mhaisalkar, J.L. Sudijono, L.C. Hsia, L. Shen,
K.Y. Zeng, Thin Solid Films 462–463 (2004) 213.
 Z. Chen, K. Prasad, C.Y. Li, P.W. Lu, S.S. Su, L.J. Tang, D. Gui, S.
Balakumar, R. Shu, R. Kumar, Appl. Phys. Lett. 84 (2004) 2442.
 A.G. Evans, J.W. Hutchinson, Acta Metall. Mater. 43 (1995) 2507.
 P.G. Charalambides, J. Lund, A.G. Evans, R.M. McMeeking, J. Appl.
Mech. 56 (1989) 77.
 D.S. Campbell, in: L.I. Maissel, R. Glang (Eds.), Handbook of Thin
Film Technology, McGraw-Hill, New York, 1970, Chap. 12.3.
 P.R. Chalker, S.J. Bull, D.S. Rickerby, Mater. Sci. Eng., A Struct.
Mater.: Prop. Microstruct. Process. 140 (1991) 583.
 R.H. Dauskardt, M. Lane, Q. Ma, N. Krishna, Eng. Fract. Mech. 61
 M.J. Bozack, Surf. Sci. Spectra 3 (1994) 82.
 A. Rajagopal, C. Gregoire, J.J. Lemaire, J.J. Pireaux, S. M.R. Baklanov,
S. Vanhaelemeersch, K. Maex, J.J. Waeterloos, J. Vac. Sci. Technol., B
17 (1999) 2336.
 C. Onneby, C.G. Pantano, J. Vac. Sci. Technol., A, Vac. Surf. Films 15
 J.W. Hutchinson, A Short Course on: the Integrity of Thin Films and
Multilayers, National University of Singapore, Singapore, 1997, p. 21.
 D. Sciti, S. Guicciardi, A. Bellosi, J. Eur. Ceram. Soc. 21 (2001) 621.
 S.J. Martin, J.P. Godschalx, M.E. Mills, E.O. Shaffer II, P.H.
Townsend, Adv. Mater. 12 (2000) 1769.
 C.S. Litteken, R.H. Dauskardt, Int. J. Fract. 119/120 (2003) 475.